LMucko/crystallography-open-database huggingface dataset:
Synthesis and Structure of the new Fluoride Bromide Ba6.668(2)Ca0.332(2)F12Br2 and Solid Solutions with Composition Ba7-xCaxF12(ClyBr1-y)2 with x = 0.5, 0 < y < 1
Fruehmann, B.; Kubel, F.; Hagemann, H.; Bill, H.; Zeitschrift fuer Anorganische und Allgemeine Chemie 630 (2004) 1484–1488; doi:

data_1537140
_publ_section_title
;
 Synthesis and Structure of the new Fluoride Bromide
 Ba6.668(2)Ca0.332(2)F12Br2 and Solid Solutions with Composition
 Ba7-xCaxF12(ClyBr1-y)2 with x = 0.5, 0 < y < 1
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              1484
_journal_page_last               1488
_journal_volume                  630
_journal_year                    2004
_chemical_formula_sum            'Ba0.5533 Br0.1667 Ca0.03 F'
_chemical_name_systematic        'Ba0.5533 Ca0.03 Br0.1667 F'
_space_group_IT_number           176
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            12
_cell_length_a                   10.5885
_cell_length_b                   10.5885
_cell_length_c                   4.2713
_cell_volume                     414.724
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Fruehmann_ZAACAB_2004_1183.cif
_cod_data_source_block           Ba0.5533Br0.1667Ca0.03F1
_cod_original_cell_volume        414.7244
_cod_original_formula_sum        'Ba0.5533 Br0.1667 Ca0.03 F1'
_cod_database_code               1537140
Crystal structure of isothiocyanato-pentaammine-cobalt(III) chloride
Kushi, Y.; Kuroya, H.; Komiyama, Y.; Nippon Kagaku Kaishi (= J.Chem.Soc.Japan) (1947-) 88 (1967) 1151–1153; doi:

data_1537141
_publ_section_title
;
 Crystal structure of isothiocyanato-pentaammine-cobalt(III) chloride
;
_journal_name_full
'Nippon Kagaku Kaishi (= J.Chem.Soc.Japan) (1947-)'
_journal_page_first              1151
_journal_page_last               1153
_journal_volume                  88
_journal_year                    1967
_chemical_formula_sum            'C H15 Cl2 Co N6 S'
_chemical_name_systematic        '(Co (N C S) (N H3)5) Cl2'
_space_group_IT_number           107
_symmetry_space_group_name_Hall  'I 4 -2'
_symmetry_space_group_name_H-M   'I 4 m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.16
_cell_length_b                   7.16
_cell_length_c                   10.13
_cell_volume                     519.321
_citation_journal_id_ASTM        NKAKB8
_cod_data_source_file            Kushi_NKAKB8_1967_739.cif
_cod_data_source_block           C1H15Cl2Co1N6S1
_cod_original_cell_volume        519.3205
_cod_original_formula_sum        'C1 H15 Cl2 Co1 N6 S1'
_cod_database_code               1537141
Doppeloxyde mit Steinsalzstruktur
Zintl, E.; Morawietz, W.; Zeitschrift fuer Anorganische und Allgemeine Chemie 245 (1940) 26–31; doi:

data_1537142
_publ_section_title
;
 Doppeloxyde mit Steinsalzstruktur
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              26
_journal_page_last               31
_journal_volume                  245
_journal_year                    1940
_chemical_formula_sum            'Na2 O3 Pr'
_chemical_name_systematic        'Na2 Pr O3'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.85
_cell_length_b                   4.85
_cell_length_c                   4.85
_cell_volume                     114.084
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Zintl_ZAACAB_1940_558.cif
_cod_data_source_block           Na2O3Pr1
_cod_original_cell_volume        114.0841
_cod_original_formula_sum        'Na2 O3 Pr1'
_cod_database_code               1537142
X-ray structure of dodecasodium tricopper(II)bis[nonatungstabismuthate(III) hydrate, a polyoxometalate salt containing α-B-BiW~9~O~33~ units
Rosu, C.; Rasu, D.; Weakley, T. J. R.; Journal of Chemical Crystallography 33 (2003) 751–755; doi:10.1023/A:1026103306556

data_1537143
_publ_section_title
;
 X-ray structure of dodecasodium tricopper(II)bis[nonatungstabismuthate(III)
 hydrate, a polyoxometalate salt containing \a-B-BiW~9~O~33~ units
;
_journal_issue                   10
_journal_name_full               'Journal of Chemical Crystallography'
_journal_page_first              751
_journal_page_last               755
_journal_paper_doi               10.1023/A:1026103306556
_journal_volume                  33
_journal_year                    2003
_chemical_formula_sum            'Bi2 Cu3 H71 Na11 O101.5 W18'
_chemical_name_systematic        'Na11 (Cu3 (H2 O)3 (Bi W9 O33)2) (H2 O)32.5'
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.63
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   33.082
_cell_length_b                   19.615
_cell_length_c                   14.885
_cell_volume                     9658.344
_citation_journal_id_ASTM        JCCYEV
_cod_data_source_file            Rosu_JCCYEV_2003_835.cif
_cod_data_source_block           H71Bi2Cu3Na11O101.5W18
_cod_original_formula_sum        'H71 Bi2 Cu3 Na11 O101.5 W18'
_cod_database_code               1537143
Crystallographic, magnetic and electric properties of rare earth chalcogenide spinels
Fujii, H.; Journal of Science of the Hiroshima University, Series A: Mathematics, Physics, Chemistry 36 (1972) 67–75; doi:

data_1537144
_publ_section_title
;
 Crystallographic, magnetic and electric properties of rare earth
 chalcogenide spinels
;
_journal_name_full
;
Journal of Science of the Hiroshima University, Series A: Mathematics, 
Physics, Chemistry
;
_journal_page_first              67
_journal_page_last               75
_journal_volume                  36
_journal_year                    1972
_chemical_formula_sum            'Cd Ho2 Se4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   11.638
_cell_length_b                   11.638
_cell_length_c                   11.638
_cell_volume                     1576.286
_citation_journal_id_ASTM        JSHAAO
_cod_data_source_file            Fujii_JSHAAO_1972_387.cif
_cod_data_source_block           Cd1Ho2Se4
_cod_original_sg_symbol_Hall     '-F 4vw 2vw 3 (x+1/8,y+1/8,z+1/8)'
_cod_original_formula_sum        'Cd1 Ho2 Se4'
_cod_database_code               1537144
Synthesis and Structure of YbPdSn2
Kussmann, D.; Poettgen, R.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (42,1987-) 56 (2001) 446–448; doi:

data_7222824
_publ_section_title
;
 Synthesis and Structure of YbPdSn2
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische 
Chemie (42,1987-)
;
_journal_page_first              446
_journal_page_last               448
_journal_volume                  56
_journal_year                    2001
_chemical_formula_sum            'Pd Sn2 Yb'
_chemical_name_systematic        'Yb Pd Sn2'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.424
_cell_length_b                   11.086
_cell_length_c                   7.384
_cell_volume                     362.144
_citation_journal_id_ASTM        ZNBSEN
_cod_data_source_file            Kussmann_ZNBSEN_2001_164.cif
_cod_data_source_block           Pd1Sn2Yb1
_cod_original_cell_volume        362.1443
_cod_original_formula_sum        'Pd1 Sn2 Yb1'
_cod_database_code               7222824
Neutron and x-ray diffraction study on polymorphism in lithium orthotantalate, Li3 Ta O4
Zocchi, M.; Gatti, M.; Santoro, A.; Roth, R.S.; Journal of Solid State Chemistry 48 (1983) 420–430; doi:

data_1537145
_publ_section_title
;
 Neutron and x-ray diffraction study on polymorphism in lithium
 orthotantalate, Li3 Ta O4
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              420
_journal_page_last               430
_journal_volume                  48
_journal_year                    1983
_chemical_formula_sum            'Li3 O4 Ta'
_chemical_name_systematic        'Li3 (Ta O4)'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 117.05
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.5
_cell_length_b                   8.5
_cell_length_c                   9.344
_cell_volume                     601.254
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Zocchi_JSSCBI_1983_211.cif
_cod_data_source_block           Li3O4Ta1
_cod_original_cell_volume        601.2543
_cod_original_formula_sum        'Li3 O4 Ta1'
_cod_database_code               1537145
Rational synthesis and X-ray structure of (Mn(II)4 (H2 O)2 (As(V) W9 O34)2)(10-) from (As(III)4 W40 O140)(28-), (Mn O4)(-) and Mn(2+)
Rosu, C.; Crans, D.C.; Weakley, T.J.R.; Polyhedron 21 (2002) 959–962; doi:

data_1537146
_publ_section_title
;
 Rational synthesis and X-ray structure of (Mn(II)4 (H2 O)2 (As(V) W9
 O34)2)(10-) from (As(III)4 W40 O140)(28-), (Mn O4)(-) and Mn(2+)
;
_journal_name_full               Polyhedron
_journal_page_first              959
_journal_page_last               962
_journal_volume                  21
_journal_year                    2002
_chemical_formula_sum            'As2 H74 K Mn4 Na9 O105 W18'
_chemical_name_systematic        'K Na9 (Mn4 (H2 O)2 (As W9 O34)2) (H2 O)35'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                98.876
_cell_angle_beta                 105.682
_cell_angle_gamma                113.29
_cell_formula_units_Z            1
_cell_length_a                   11.6368
_cell_length_b                   14.2113
_cell_length_c                   17.6343
_cell_volume                     2463.886
_citation_journal_id_ASTM        PLYHDE
_cod_data_source_file            Rosu_PLYHDE_2002_434.cif
_cod_data_source_block           H74As2K1Mn4Na9O105W18
_cod_original_formula_sum        'H74 As2 K1 Mn4 Na9 O105 W18'
_cod_database_code               1537146
Crystallographic, Magnetic and Electric Properties of Rare Earth Chalcogenide Spinels
Fujii, H.; Journal of Science of the Hiroshima University, Series A: Mathematics, Physics, Chemistry 36 (1972) 67–75; doi:

data_1537147
_publ_section_title
;
 Crystallographic, Magnetic and Electric Properties of Rare Earth
 Chalcogenide Spinels
;
_journal_name_full
;
Journal of Science of the Hiroshima University, Series A: Mathematics, 
Physics, Chemistry
;
_journal_page_first              67
_journal_page_last               75
_journal_volume                  36
_journal_year                    1972
_chemical_formula_sum            'Cd Ho2 S4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   11.24
_cell_length_b                   11.24
_cell_length_c                   11.24
_cell_volume                     1420.035
_citation_journal_id_ASTM        JSHAAO
_cod_data_source_file            Fujii_JSHAAO_1972_388.cif
_cod_data_source_block           Cd1Ho2S4
_cod_original_sg_symbol_Hall     '-F 4vw 2vw 3 (x+1/8,y+1/8,z+1/8)'
_cod_original_formula_sum        'Cd1 Ho2 S4'
_cod_database_code               1537147
The crystal structure of Li2 Ba P2 O7
Kutoglu, A.; Allmann, R.; Nikolov, V.; Petrov, K.; Private Communication 2003 (2003) 1–1; doi:

data_1537148
_publ_section_title
;
 The crystal structure of Li2 Ba P2 O7
;
_journal_name_full               'Private Communication'
_journal_page_first              1
_journal_page_last               1
_journal_volume                  2003
_journal_year                    2003
_chemical_formula_sum            'Ba Li2 O7 P2'
_chemical_name_systematic        'Li2 Ba (P2 O7)'
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_Hall           '-A 2ya'
_space_group_name_H-M_alt        'A 1 2/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.7
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   13.865
_cell_length_b                   12.163
_cell_length_c                   7.087
_cell_volume                     1195.062
_citation_journal_id_ASTM        PRICO6
_cod_data_source_file            Kutoglu_PRICO6_2003_1745.cif
_cod_data_source_block           Ba1Li2O7P2
_cod_depositor_comments
;
 Updating space group information.

 Antanas Vaitkus,
 2018-07-23
;
_cod_original_formula_sum        'Ba1 Li2 O7 P2'
_cod_database_code               1537148
Structure and conductivity of zirconium-doped polycristalline lithium yttrium oxide
Zou, Y.; Petric, A.; Materials Research Bulletin 28 (1993) 1169–1175; doi:

data_1537149
_publ_section_title
;
 Structure and conductivity of zirconium-doped polycristalline lithium
 yttrium oxide
;
_journal_name_full               'Materials Research Bulletin'
_journal_page_first              1169
_journal_page_last               1175
_journal_volume                  28
_journal_year                    1993
_chemical_formula_sum            'Li0.9 O2 Y0.9 Zr0.1'
_chemical_name_systematic        'Li0.9 (Zr0.1 Y0.9) O2'
_space_group_IT_number           141
_symmetry_space_group_name_Hall  'I 4bw 2bw -1bw'
_symmetry_space_group_name_H-M   'I 41/a m d :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.388
_cell_length_b                   4.388
_cell_length_c                   10.6
_cell_volume                     204.098
_citation_journal_id_ASTM        MRBUAC
_cod_data_source_file            Zou_MRBUAC_1993_923.cif
_cod_data_source_block           Li0.9O2Y0.9Zr0.1
_cod_original_cell_volume        204.0982
_cod_original_sg_symbol_Hall     '-I 4bd 2 (x+1/2,y+1/4,z+1/8)'
_cod_database_code               1537149
Rational synthesis and X-ray structure of (Mn(II)4 (H2 O)2 (As(V) W9 O34)2)(10-) from (As(III)4 W40 O140)(28-), (Mn O4)(-) and Mn(2+)
Rosu, C.; Crans, D.C.; Weakley, T.J.R.; Polyhedron 21 (2002) 959–962; doi:

data_1537150
_publ_section_title
;
 Rational synthesis and X-ray structure of (Mn(II)4 (H2 O)2 (As(V) W9
 O34)2)(10-) from (As(III)4 W40 O140)(28-), (Mn O4)(-) and Mn(2+)
;
_journal_name_full               Polyhedron
_journal_page_first              959
_journal_page_last               962
_journal_volume                  21
_journal_year                    2002
_chemical_formula_sum            'As4 H112 K Na27 O196 W40'
_chemical_name_systematic        'K Na27 (As4 W40 O140) (H2 O)56'
_space_group_IT_number           82
_symmetry_space_group_name_Hall  'I -4'
_symmetry_space_group_name_H-M   'I -4'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   19.491
_cell_length_b                   19.491
_cell_length_c                   25.783
_cell_volume                     9794.938
_citation_journal_id_ASTM        PLYHDE
_cod_data_source_file            Rosu_PLYHDE_2002_435.cif
_cod_data_source_block           H112As4K1Na27O196W40
_cod_original_formula_sum        'H112 As4 K1 Na27 O196 W40'
_cod_database_code               1537150
Crystallographic, magnetic and electric properties of rare earth chalcogenide spinels
Fujii, H.; Journal of Science of the Hiroshima University, Series A: Mathematics, Physics, Chemistry 36 (1972) 67–75; doi:

data_1537151
_publ_section_title
;
 Crystallographic, magnetic and electric properties of rare earth
 chalcogenide spinels
;
_journal_name_full
;
Journal of Science of the Hiroshima University, Series A: Mathematics, 
Physics, Chemistry
;
_journal_page_first              67
_journal_page_last               75
_journal_volume                  36
_journal_year                    1972
_chemical_formula_sum            'Cd Er2 Se4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   11.603
_cell_length_b                   11.603
_cell_length_c                   11.603
_cell_volume                     1562.107
_citation_journal_id_ASTM        JSHAAO
_cod_data_source_file            Fujii_JSHAAO_1972_389.cif
_cod_data_source_block           Cd1Er2Se4
_cod_original_sg_symbol_Hall     '-F 4vw 2vw 3 (x+1/8,y+1/8,z+1/8)'
_cod_original_formula_sum        'Cd1 Er2 Se4'
_cod_database_code               1537151
The rutile structure of Al1-x()xO1-3xF1+3x, x=0.0886
Kutoglu, A.; Zeitschrift fuer Kristallographie (149,1979-) 199 (1992) 197–201; doi:

data_8104202
_publ_section_title
;
 The rutile structure of Al1-x()xO1-3xF1+3x, x=0.0886
;
_journal_name_full
'Zeitschrift fuer Kristallographie (149,1979-)'
_journal_page_first              197
_journal_page_last               201
_journal_volume                  199
_journal_year                    1992
_chemical_formula_sum            'Al0.9114 F1.2658 O0.7342'
_chemical_name_systematic        'Al0.9114 O0.7342 F1.2658'
_space_group_IT_number           136
_symmetry_space_group_name_Hall  '-P 4n 2n'
_symmetry_space_group_name_H-M   'P 42/m n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.627
_cell_length_b                   4.627
_cell_length_c                   3.005
_cell_volume                     64.334
_citation_journal_id_ASTM        ZEKRDZ
_cod_data_source_file            Kutoglu_ZEKRDZ_1992_36.cif
_cod_data_source_block           Al0.9114F1.2658O0.7342
_cod_original_cell_volume        64.33443
_cod_database_code               8104202
Neutron scattering study of the niobium monoxide intergrowth phases in niobium bronze.
Zubkov, V.G.; Perelyaev, V.A.; Berger, I.F.; Shveikin, G.P.; Voronin, V.I.; Kontsevaya, I.A.; Doklady Akademii Nauk SSSR 312 (1990) 615–618; doi:

data_1537152
_publ_section_title
;
 Neutron scattering study of the niobium monoxide intergrowth phases in
 niobium bronze.
;
_journal_name_full               'Doklady Akademii Nauk SSSR'
_journal_page_first              615
_journal_page_last               618
_journal_volume                  312
_journal_year                    1990
_chemical_formula_sum            'Ba Nb4 O5.48'
_space_group_IT_number           123
_symmetry_space_group_name_Hall  '-P 4 2'
_symmetry_space_group_name_H-M   'P 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.189
_cell_length_b                   4.189
_cell_length_c                   8.221
_cell_volume                     144.260
_citation_journal_id_ASTM        DANKAS
_cod_data_source_file            Zubkov_DANKAS_1990_1065.cif
_cod_data_source_block           Ba1Nb4O5.48
_cod_original_cell_volume        144.2598
_cod_original_formula_sum        'Ba1 Nb4 O5.48'
_cod_database_code               1537152
Deuterium site occupation in the oxygen-stabilized eta-carbides Zr3 V3 O Dx: Preparation and neutron powder diffraction
Rotella, F.J.; Jorgensen, J.D.; Flotow, H.E.; Gruen, D.M.; Journal of Chemical Physics 79 (1983) 4522–4531; doi:

data_1537153
_publ_section_title
;
 Deuterium site occupation in the oxygen-stabilized eta-carbides Zr3 V3 O
 Dx: Preparation and neutron powder diffraction
;
_journal_name_full               'Journal of Chemical Physics'
_journal_page_first              4522
_journal_page_last               4531
_journal_volume                  79
_journal_year                    1983
_chemical_formula_sum            'D1.86 O V3 Zr3'
_chemical_name_systematic        'Zr3 V3 O D1.86'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            16
_cell_length_a                   12.3175
_cell_length_b                   12.3175
_cell_length_c                   12.3175
_cell_volume                     1868.821
_citation_journal_id_ASTM        JCPSA6
_cod_data_source_file            Rotella_JCPSA6_1983_663.cif
_cod_data_source_block           D1.86O1V3Zr3
_cod_original_sg_symbol_Hall     '-F 4vw 2vw 3 (x+1/8,y+1/8,z+1/8)'
_cod_original_formula_sum        'D1.86 O1 V3 Zr3'
_cod_database_code               1537153
Crystallographic, magnetic and electric properties of rare earth chalcogenide spinels
Fujii, H.; Journal of Science of the Hiroshima University, Series A: Mathematics, Physics, Chemistry 36 (1972) 67–75; doi:

data_1537154
_publ_section_title
;
 Crystallographic, magnetic and electric properties of rare earth
 chalcogenide spinels
;
_journal_name_full
;
Journal of Science of the Hiroshima University, Series A: Mathematics, 
Physics, Chemistry
;
_journal_page_first              67
_journal_page_last               75
_journal_volume                  36
_journal_year                    1972
_chemical_formula_sum            'Cd Er2 S4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   11.192
_cell_length_b                   11.192
_cell_length_c                   11.192
_cell_volume                     1401.920
_citation_journal_id_ASTM        JSHAAO
_cod_data_source_file            Fujii_JSHAAO_1972_390.cif
_cod_data_source_block           Cd1Er2S4
_cod_original_cell_volume        1401.92
_cod_original_sg_symbol_Hall     '-F 4vw 2vw 3 (x+1/8,y+1/8,z+1/8)'
_cod_original_formula_sum        'Cd1 Er2 S4'
_cod_database_code               1537154